Transition metal oxides (TMOs) have attracted extensive research attentions as promising electrocatalytic materials. Despite low cost and high stability, the electrocatalytic activity of TMOs still cannot satisfy the requirements of applications. Inspired by kinetics, the design of hollow porous structure is considered as a promising strategy to achieve superior electrocatalytic performance. In this work, cubic NiO hollow porous architecture (NiO HPA) was constructed through coordinating etching and precipitating (CEP) principle followed by post calcination. Being employed to detect glucose, NiO HPA electrode exhibits outstanding electrocatalytic activity in terms of high sensitivity (1323 μA mM−1 cm−2) and low detection limit (0.32 μM). The excellent electrocatalytic activity can be ascribed to large specific surface area (SSA), ordered diffusion channels, and accelerated electron transfer rate derived from the unique hollow porous features. The results demonstrate that the NiO HPA could have practical applications in the design of nonenzymatic glucose sensors. The construction of hollow porous architecture provides an effective nanoengineering strategy for high-performance electrocatalysts.
Detection of glucose with fast, accurate, and low-cost process is importance for clinical biochemistry, pharmaceutical analysis, food industry, and environmental monitoring [1,2,3]. Among the multitudinous techniques, electrochemical detection has been considered as one of the most convenient approach owing to its high sensitivity, low cost, and attractive lower detection limit [4,5,6]. However, the common glucose oxidase-based electrochemical sensors are restricted by the drawback of insufficient stability originating from the nature of enzymes [7,8,9]. To address these issues, earth-abundant electrocatalysts based on TMOs were recommended due to their lower cost, physicochemical stability, and redox electroactivity [10,11,12]. However, the overall electrocatalytic activity of conventional TMOs is still far away from the requirements of applications. It is still a challenge to rationally design high-active TMO electrocatalysts for glucose.
Generally, the process of kinetics plays a decisive role in electrocatalytic activity for established electrocatalytic materials. Inspired by the intimate connection between kinetics and microstructures, improved electrocatalytic activity can be achieved by the engineering of microstructures, including surface area, pore structure, and architecture features [13, 14]. The porous structure offers large specific surface area (SSA) and provides amounts of active sites. Furthermore, the porous structure also affords enough diffusion channels for analyte and intermediate products, which are beneficial for mass transport process [15, 16]. On the other hand, hollow structures combining functional shells and inner voids can offer larger electrolyte-electrode contact area and reduce the length for both mass and electron transport . Furthermore, the available inner cavities effectively prevent electroactive nanoparticles from aggregation and accommodate the volume change and structural strain accompanied with repeated measurements . In conclusion, high-active TMO electrocatalysts can be acquired through the design of hollow porous architecture.
As a typical transition metal oxide, NiO was reported as an efficient catalyst for electrooxidation of glucose due to the redox couple of Ni3+/Ni2+ in alkaline medium, implying potential applications in electrochemical glucose sensor. In this work, cubic NiO HPA was constructed through a Cu2O-templated coordinating etching and precipitating (CEP) method and post calcination. The hollow porous structure provides large SSA, well-defined interior voids, abundant ordered transfer channels, and high electron transfer efficiency. Being employed to detect glucose, NiO HPA electrode presents higher sensitivity and lower detection limit compared to broken NiO HPA (NiO BHPA), demonstrating advantages of the hollow porous architecture. This facile strategy to construct hollow porous architecture provides a valid method in the development of highly efficient nanomaterials for electrochemical sensors.
CuCl2·2H2O, NiCl2·6H2O, Na2S2O3·5H2O, polyvinylpyrrolidone (PVP, Mw = 40,000), and NaOH were purchased from Chengdu Kelong. Glucose (Glu.), lactose (Lact.), sucrose (Sucr.), fructose (Fruc.), L-ascorbic acid (AA), uric acid (UA), and Nafion solution (5 wt% in mixture of lower aliphatic alcohols and water) were purchased from Sigma-Aldrich without further purification.
Synthesis of Cu2O Template
The cubic Cu2O templates were synthesized according to our previous work . In this typical procedure, 20 ml NaOH (2 M) was added dropwise into 200 mL CuCl2·2H2O (10 mM) under stirring at 55 °C. After 0.5 h, 4 mL AA (0.6 M) was introduced dropwise into the above solution. The suspension was further aged for 3 h and washed with water several times by centrifugation. The XRD pattern and SEM and TEM images are shown in Additional file 1: Figure S1.
Synthesis of NiO HPA
NiO HPA was synthesized by a CEP method. First, Cu2O (10 mg) and NiCl2·6H2O (3 mg) were dispersed into 10 mL ethanol-water mixed solvent (volume ratio = 1:1) for 7 min by ultrasonication. Then, PVP (0.33 g) was added into the solution with vigorous agitation for 30 min. Four milliliters Na2S2O3 (1 M) was dropped into the system; the reaction was proceeded at room temperature for 3 h until the color of the suspension changed from red to light green. The Ni(OH)2 precursor was washed several times by warm ethanol-water and dried at room temperature. Finally, NiO HPA was successively obtained under an air atmosphere at 400 °C for 2 h with a slow ramp rate of 1 °C/min. NiO BHPA was obtained through strong ultrasonic treatment of NiO HPA for 2 h.
The composition and structure of the products were characterized by X-ray diffraction (XRD, Rigaku D/Max-2400). The composition was further analyzed by the X-ray photoelectron spectroscopy (XPS, ESCALAB250Xi) with the C 1s peaks at 284.8 eV as an internal standard. The morphologies and microstructures of the products were observed using field emission scanning electron microscope (FESEM, FEI Quanta 250, Zeiss Gemini 500) and high-resolution transmission electron microscope (HRTEM, FEI F20). Brunauer-Emmett-Teller (BET, Belsort-max) was applied to analyze the specific surface area and pore structure.
All electrochemical measurements were operated in 0.1 M NaOH on μIII Autolab electrochemical workstation. A three-electrode configuration with NiO HPA (or NiO BHPA) modified glassy carbon electrode (GCE, Ф = 3 mm) as the working electrodes and Ag/AgCl (in saturated KCl) and platinum disk electrode (Ф = 2 mm) as the reference electrode and counter electrode, respectively. Typically, GCE was polished with alumina slurry (3, 0.5, and 0.05 μm). Then, the NiO HPA (10 mg) was dissolved into a mixture of 0.1 mL Nafion and 0.9 mL distilled water. Finally, 5 μL of the mixture was dropped onto the pretreated GCE (70.77 μg/cm2) and dried at room temperature. NiO BHPA-modified GCE was also prepared under the same condition to verify the advantages of NiO HPA. The modified electrodes were measured by cyclic voltammetry (CV), chronoamperometry (CA), and electrochemical impedance spectroscopy (EIS) to evaluate its electrocatalytic activity. EIS measurements were carried out over the frequency range between 0.01–100 kHz with a perturbation amplitude of 5 mV versus the open-circle potential.
Results and Discussion
As shown in Fig. 1a, the diffraction peaks located at 37.21°, 43.27°, 62.87°, and 75.42° correspond to (111), (200), (220), and (311) facets of face-centered cubic NiO (JCPDS.no.47-1049) . There are no other diffraction peaks, indicating the purity of the products. XPS was further employed to analyze the element composition and oxidation state of NiO HPA. The survey spectrum (Fig. 1b) demonstrates O 1s and Ni 2p peaks at 531.5 and 855.7 eV, respectively, revealing main elements of the products. In the Ni 2p spectrum (Fig. 1c, see fitting lines in Additional file 1: Table S1), two major peaks located at 855.8 eV (Ni 2p3/2) and 873.5 eV (Ni 2p1/2) with a spin-energy separation of 17.7 eV are clearly investigated, which is the feature of NiO phase . The satellite peaks of Ni 2p3/2 and Ni 2p1/2 are located at around 861.5 and 880.0 eV, respectively. From Fig. 1d (see fitting lines in Additional file 1: Table S2), the fitting peak of O1 at 529.8 eV is the Ni–O bond in Ni–OH species. O2 peak at a binding energy of 831.3 eV is usually associated with chemisorbed oxygen, hydroxyls, and under-coordinated lattice oxygen. The peak of O3 at 532.7 eV is the multiplicity of physi- and chemisorbed water on/near the surface [22,23,24]. The analysis of XPS and XRD confirm the successful preparation of NiO.
The morphologies of Ni(OH)2 precursor (Additional file 1: Figure S2) and NiO HPA (Fig. 2) were clearly observed by SEM and TEM. The SEM images (Fig. 2a, b) of as-obtained NiO present uniform cubic feature with an edge length about 600 nm. From Fig. 2c, it is clearly observed that the rough shell of NiO HPA consists of amounts of interconnected fine particles. As shown in Fig. 2d, the border of NiO products is black and the interior is translucent. Combing with the SEM observations in Fig. 2a–c, the cubic hollow characteristics of the NiO products can be confirmed. As displayed in Fig. 2e, the shell thickness of the cube is about 40 nm, which is thinner than that of Ni(OH)2 precursor (about 60 nm). The shrink of shell thickness is attributed to the loss of H2O in the precursor after heat treatment. In Fig. 2f, the spacing for marked adjacent lattice fringes are about 0.21 and 0.24 nm, respectively, corresponding to (200) and (111) facets of NiO. The selected area electron diffraction (SAED) rings can be indexed to (111), (200), and (220) facets of NiO inside and out, which agrees well with the XRD results . In addition, the elemental mapping images in Fig. 2g exhibit surface rich distribution of Ni and O. As shown in Fig. 2h, the line-scan EDX profile demonstrates the uniform near-surface distribution of O and Ni, reconfirming the hollow architecture. NiO HPA would provide enough active sites and abundant diffusion channels, which favor the mass transfer process for electrolyte and glucose. Furthermore, the thin shell of NiO HPA apparently shortens the transfer distance of electrons and accelerates the transfer rate, endowing NiO HPA with promising electrocatalytic activity.
In order to understand the relevant formation mechanism, the precipitate prepared at 0, 10, 20, 30, and 180 min were collected and observed by TEM. As shown in Fig. 3a, the solid cubic Cu2O crystal has an edge length about 600 nm. With the introduction of S2O32−, the coordinating etching of Cu2O preferentially occurs at the corner due to higher diffusion intensity . As the reaction proceed, the interior Cu2O templates significantly shrink to octahedron-like structure until completely removed. As observed in Fig. 3b, the color of the reaction system gradually becomes shallow and the light green precipitates generate at the same time. Combined with TEM results, the overall CEP route and formation mechanism were illustrated in Fig. 3c. The CEP mechanism can be described as follows: (i) Cu+ prefers to form soluble [Cu2(S2O32−) x ]2 − 2x complex through the combination with S2O32− (reaction (1)) and simultaneously OH− is released; (ii) The partly hydrolyzation of S2O32− promotes the supply of OH− (reaction (2)). (iii) Reactions (1) and (2) synchronously drive reaction (3) from left to right, facilitating the formation of Ni(OH)2 shell . Regarding kinetics factors, the etching rate of Cu2O depends on the diffusion of S2O32− from exterior into internal space and the growth rate of Ni(OH)2 shell is correlated to the transport of OH− from interior to exterior . Synchronously controlling of etching rate towards Cu2O and precipitating rate of Ni(OH)2 shell leads to the formation of well-defined hollow Ni(OH)2 precursor. NiO HPA is finally obtained through the post calcination of Ni(OH)2 precursor.
The surface area and porosity of NiO HPA and NiO BHPA (Additional file 1: Figure S3) were also characterized by BET method. NiO HPA possesses SSA of 27.08 m2/g and a pore volume of 0.087 cm3/g (Fig. 4a), which is much larger than the reported NiO materials . Regarding the pore size distribution, NiO HPA mainly presents a concentrated distribution at around 7 nm, which is related to the ordered channels between NiO nanoparticles. The large SSA and ordered channels can effectively improve the absorption of analyte and mass transport process, leading to enhanced electrocatalytic activity. The SSA and pore volume of the broken sample are 5.24 m2/g and 0.078 cm3/g (Fig. 4b), respectively, which is much smaller than those of NiO HPA. This can be attributed to the collapse of original hollow structure after ultrasonic treatment. Notably, no concentrated pore distribution is observed for NiO BHPA (inset of Fig. 4b), indicating complete destruction of ordered diffusion channels. The decrease of SSA and destruction of ordered diffusion channels are adverse for kinetics, which may result in poor electrocatalytic activity. Accordingly, NiO HPA possesses beneficial microstructures for electrocatalysis compared to the broken samples.
Figure 5a shows the CVs of NiO HPA and NiO BHPA electrodes with and without 1 mM glucose. A pair of well-defined peaks located at 0.48 and 0.38 V are clearly investigated in curve III, which are related to Ni2+/Ni3+ redox couple. The redox peak current of curve III is obviously higher than that of curve I. This is related to the collapse of hollow architecture and the decrease of SSA. Upon the addition of glucose, current responses are clearly observed on both electrodes (curve II and IV). NiO HPA electrode exhibits higher current response than that of NiO BHPA electrode. In addition, the onset potential for electrooxidation of glucose on NiO HPA electrode (0.43 V) is lower than that of NiO BHPA electrode (0.46 V), revealing higher electrocatalytic activity. The high electrocatalytic activity is attributed to large amounts of active sites, ordered pore structure, and high electron transfer rate provided by the hollow porous structure. The electrooxidation of glucose on NiO HPA electrode is driven by Ni2+/Ni3+ redox couple in alkaline medium according to the following reactions [30, 31]:
As shown above, OH− plays an important role in the electrocatalytic reaction. Obviously, alkaline medium accelerates the redox of Ni2+/Ni3+ compared to neutral medium (Additional file 1: Figure S4), leading to higher electrocatalytic activity.
Nyquist plots of NiO HPA and NiO BHPA electrodes were displayed in Fig. 5b. Each plot is characterized by a semicircle in the high-frequency region and a straight line in the low-frequency region. Generally, the intercept on the real axis represents the solution resistance (Rs), which is composed of intrinsic resistance, ionic resistance, and contact resistance. The semicircle diameter related to electron transfer resistance is represented by Rct. As shown in Additional file 1: Table S3, NiO HPA electrode exhibits smaller Rs and Rct than NiO BHPA. The facts can be attributed to the beneficial electron transfer kinetics derived from the hollow feature. The slope of the impedance plot in the low frequency range corresponds to the Warburg impedance (Zw), which represents the diffusive resistance . It is clear that NiO HPA favors the diffusion kinetics; however, the NiO BHPA hinders the diffusion of electrolyte. This can be ascribed to the destruction of the ordered diffusion channels after ultrasonic. On the basis of above EIS discussions, NiO HPA electrode is more beneficial for both electron and mass transfer kinetics compared to the broken sample, implying the advantages of NiO HPA as an electrocatalyst for glucose.
The kinetics of NiO HPA electrode was determined from the CVs with different scan rates in 1 mM glucose solution (Fig. 5c). As depicted in Fig. 5d, the anodic and cathodic peak currents are proportional to the square root of scan rates, demonstrating a typical diffusion-controlled dynamic process. Furthermore, no significant positive/negative shift is observed for anodic/cathodic peak, implying unimpeded diffusion kinetics originated from the hollow porous structure.
The Selectivity, Reproducibility, and Stability of NiO HPA Electrode
To obtain optimized working potential, current response of glucose and interference of AA were taken into consideration under different potentials and the data were displayed in Fig. 6a. From the statistical data in Fig. 6b, 0.6 V was selected by the fact that NiO HPA electrode exhibits maximum current response to glucose and minimum interference to AA at 0.6 V. Figure 6c displays the typical amperometric responses of NiO HPA and NiO BHPA towards different concentration of glucose at 0.6 V. Notable current responses are clearly observed for the two electrodes, and the current responses increase with the glucose concentration increasing. Figure 6d presents the relationship between response currents and glucose concentration for NiO HPA and NiO BHPA electrodes. NiO HPA electrode presents a linear range from 0.32 to 1100 μM with a sensitivity of 1323 μA mM−1 cm−2, which is higher than that of NiO BHPA electrode (753 μA mM−1 cm−2). Moreover, the limit of detection (LOD) of NiO HPA electrode (0.32 μM) is much lower than that of NiO BHPA (14.2 μM). To manifest the advantages of NiO HPA, the performance of NiO HPA electrode was compared with other reported NiO-based glucose detection electrodes in Table 1. It is found that NiO HPA electrode presents satisfying electrocatalytic activity towards glucose in terms of high sensitivity and low LOD, indicating potential applications in electrochemical glucose sensors. This is essentially attributed to the abundant active sites, faster mass transport kinetics, and accelerated electron transfer kinetics derived from the highly porous hollow architecture.
Selectivity is an important indicator to assess the performance of glucose sensors. Some easily oxidized compounds, such as Lact., Sucr., Fruc., UA, and AA normally co-existed with glucose in human blood. Notably, the physiological level of these interfering species is more or less one tenth of the glucose concentration . Thus, the selectivity of NiO HPA electrode was evaluated by introducing 0.01 mM above interfering species during amperometric measurement towards 0.1 mM glucose. As shown in Fig. 7a, no severe interference is observed for Lact., Sucr., Fruc., and UA. The major interfering species AA only exhibit 8.7% interference current towards glucose. Furthermore, the second addition of 50 μM glucose still retains about (89 ± 0.2)% of its original response, indicating excellent anti-interference performance. The outstanding selectivity could be attributed to the electrostatic repelling effect between NiO HPA electrode and interfering species. NiO HPA electrode would be negatively charged in 0.1 M NaOH because the pH of electrolyte is above the isoelectric point of NiO . In addition, the major interfering species (AA) is easy to lose protons in alkaline solution and possess a negatively charged shell . The electrostatic repulsion between the shell of interferent and NiO HPA electrode leads to improved selectivity. The stability of NiO HPA electrode was estimated by measuring its current responses towards 0.1 mM glucose over 30 days. In Fig. 7b, the current response still retains 83.13% of its initial response after 30 days, revealing excellent long-term stability of NiO HPA electrode at room temperature. The current response of NiO HPA electrode towards 0.1 mM glucose is stable over an operation time of 2000 s with a loss of 9.82% of its original response. The five independently prepared NiO HPA electrodes exhibit an acceptable RSD of 3.12% for current responses towards 0.1 mM glucose at 0.6 V. Moreover, current responses for a same NiO HPA electrode towards 0.1 mM glucose were measured for ten times and the current responses display a RSD of 2.36%, demonstrating remarkable reproducibility. The NiO HPA electrode expresses high sensitivity, excellent stability, and remarkable reproducibility, making it attractive for practical applications.
Detection of Glucose in Human Serum
NiO HPA electrode was further applied to detect glucose level in human blood, and the results were compared with a medical equipment (Table 2). The serums samples were provided by a local hospital and diluted with alkaline electrolytes before measurements [36, 37]. The response current measured at 0.6 V was recorded to calculate corresponding glucose concentration according to working equation. NiO HPA electrode shows a RSD of 2.85% towards detection of glucose. In addition, NiO HPA electrode presents accredited recovery between 92 and 102%, demonstrating excellent practicability in the determination of glucose in human serum.
In summary, we have successfully fabricated a NiO HPA electrocatalyst for glucose through a CEP method. The NiO HPA offers large SSA, ordered pore structure, and short electronic transfer route, which are beneficial for electrocatalytic kinetics. As a nonenzymatic glucose detection electrode, NiO HPA exhibits higher sensitivity of 1323 μA mM−1 cm−2 and lower LOD of 0.32 μM compared to NiO BHPA. In the term of selectivity, less than 8.7% interference is investigated for the common interfering species. Simultaneously, NiO HPA electrode retains 89.02% of its original response after 30 days. In addition, the designed NiO HPA was successfully applied to detect glucose in human serum. NiO HPA presents accredited stability and practicability compared to medical equipment. The design of hollow porous architecture paves a high efficient way to obtain low cost and high-performance electrocatalysts for glucose.
Nai JW, Wang SQ, Bai Y, Guo L (2013) Amorphous Ni(OH)2 nanoboxes: fast fabrication and enhanced sensing for glucose. Small 9:3147-3152
Noh HB, Lee KS, Chandra P, Won MS, Shim YB (2012) Application of a Cu-Co alloy dendrite on glucose and hydrogen peroxide sensors. Electrochim Acta 61:36–43
Wang MQ, Ye C, Bao SJ, Xu MW, Zhang Y, Wang L, Ma XQ, Guo J, Li CM (2017) Nanostructured cobalt phosphates as excellent biomimetic enzymes to sensitively detect superoxide anions released from living cells. Biosens Bioelectron 87:998–1004
Bao SJ, Li CM, Zang JF, Cui XQ, Qiao Y, Guo J (2008) New nanostructured TiO2 for direct electrochemistry and glucose sensor applications. Adv Funct Mater 18:591–599
Wang J (2008) Electrochemical glucose biosensors. Chem Rev 108:814–825
Gouveia-Carida C, Pauliukaite R, Brett CMA (2008) Development of electrochemical oxidase biosensors based on carbon nanotube-modified carbon film electrodes for glucose and ethanol. Electrochim Acta 53:6732–6739
Kang X, Mai Z, Zou X, Cai P, Mo J (2007) A sensitive nonenzymatic glucose sensor in alkaline media with a copper nanocluster/multiwall carbon nanotube-modified glassy carbon electrode. Anal Biochem 363:143–150
Feng D, Wang F, Chen ZL (2009) Electrochemical glucose sensor based on one-step construction of gold nanoparticle–chitosan composite film. Sensors Actuators B 138:539–544
Başkaya G, Yıldız Y, Savk A, Okyay TO, Eriş S, Sert H, Şen F (2017) Rapid, sensitive and reusable detection of glucose by highly monodisperse nickel nanoparticles decorated functionalized multi-walled carbon nanotubes. Biosens Bioelectron 91:728–733
Chen C, Xie QJ, Yang DW, Xiao HL, Fu YC, Tan YM, Yao SZ (2013) Recent advances in electrochemical glucose biosensors: a review. RSC Adv 3:4473–4491
Heller A, Feldman B (2008) Electrochemical glucose sensors and their applications in diabetes management. Chem Rev 108:2482–2505
Scognamiglio V (2013) Nanotechnology in glucose monitoring: advances and challenges in the last 10 years. Biosens Bioelectron 47:12–25
Kaneti YV, Tang J, Salunkhe RR, Jiang XC, Yu A, Wu KCW, Yamauchi Y (2017) Nanoarchitectured design of porous materials and nanocomposites from metal-organic frameworks. Adv Mater 29:1604898–1604938
Xu Y, Tu WG, Zhang BW, Yin SM, Huang YZ, Kraft M, Xu R (2017) Nickel nanoparticles encapsulated in few-layer nitrogen-doped graphene derived from metal-organic frameworks as efficient bifunctional electrocatalysts for overall water splitting. Adv Mater 29:1605957–1605965
Bak SM, Kim KH, Lee CW, Kim KB (2011) Mesoporous nickel/carbon nanotube hybrid material prepared by electroless deposition. J Mater Chem 21:1984–1990
Liu H, Wang GX, Liu J, Qiao SZ, Ahnc H (2011) Highly ordered mesoporous NiO anode material for lithium ion batteries with an excellent electrochemical performance. J Mater Chem 21:3046–3052
Ci SQ, Huang TZ, Wen ZH, Cui SM, Mao S, Steeber DA, Chen JH (2014) Nickel oxide hollow microsphere for non-enzyme glucose detection. Biosens Bioelectron 54:251–257
Cao CY, Guo W, Cui ZM, Song WG, Cai W (2011) Microwave-assisted gas/liquid interfacial synthesis of flowerlike NiO hollow nanosphere precursors and their application as supercapacitor electrodes. J Mater Chem 21:3204–3209
Tian LL, Zhong XH, Hu WP, Liu BT, Li YF (2014) Fabrication of cubic PtCu nanocages and their enhanced electrocatalytic activity towards hydrogen peroxide. Nanoscale Res Lett 9:1–5
Kim SI, Lee JS, Ahn HJ, Song HK, Jang JH (2013) Facile route to an efficient NiO supercapacitor with a three-dimensional nanonetwork morphology. ACS Appl Mater Interfaces 5:1596–1603
Liang K, Tang XZ, Hu WC (2012) High-performance three-dimensional nanoporous NiO film as a supercapacitor electrode. J Mater Chem 22:11062–11067
Chigane M, Ishikawa M (1998) XRD and XPS characterization of electrochromic nickel oxide thin films prepared by electrolysis-chemical deposition. J Chem Soc Faraday Trans 94:3665–3670
Biesinger MC, Payne BP, Lau LWM, Gerson A, Smart RSC (2009) X-ray photoelectron spectroscopic chemical state quantification of mixed nickel metal, oxide and hydroxide systems. Surf Interface Anal 41:324–332
Varghese B, Reddy MV, Wu ZY, Lit CS, Hoong TC, Rao GVS, Chowdari BVR, Wee ATS, Lim CT, Sow CH (2008) Fabrication of NiO nanowall electrodes for high performance lithium ion battery. Chem Mater 20:3360–3367
Zhu H, Gu L, Yu D, Sun YJ, Wan M, Zhang M, Wang L, Wu WW, Yao JM, ML D, Guo SJ (2017) The marriage and integration of nanostructures with different dimensions for synergistic electrocatalysis. Energy Environ Sci 10:321–330
Bao HZ, Zhang ZH, Hua Q, Huang WX (2014) Compositions, structures and catalytic activities of CeO2@Cu2O nanocomposites prepared by the template-assisted method. Langmuir 30:6427–6436
Sun SD, Yang ZM (2014) Cu2O-templated strategy for synthesis of definable hollow architectures. Chem Commun 50:7403–7415
Sohn JH, Cha HG, Kim CW, Kim DK, Kang YS (2013) Fabrication of hollow metal oxide nanocrystals by etching cuprous oxide with metal(II) ions: approach to the essential driving force. Nano 5:11227–11233
Yang P, Tong XL, Wang GZ, Gao Z, Guo XY, Qin Y (2015) NiO/SiC nanocomposite prepared by atomic layer deposition used as a novel electrocatalyst for non-enzymatic glucose sensing. ACS Appl Mater Interfaces 7:4772–4778
Li M, Bo XJ, Mu ZC, Zhang YF, Guo LP (2014) Electrodeposition of nickel oxide and platinum nanoparticles on electrochemically reduced graphene oxide film as a nonenzymatic glucose sensor. Sensors Actuators B 192:261–268
Safavi A, Maleki N, Farjami E (2009) Fabrication of a glucose sensor based on a novel nanocomposite electrode. Biosens Bioelectron 24:1655–1660
Wu CH, Deng SX, Wang H, Sun YX, Liu JB, Yan H (2014) Preparation of novel three-dimensional NiO/Ultrathin derived graphene hybrid for supercapacitor applications. ACS Appl Mater Interfaces 6:1106–1112
Kong CC, Tang LL, Zhang XZ, Sun SD, Yang SC, Song XP, Yang ZM (2014) Templating synthesis of hollow CuO polyhedron and its application for nonenzymatic glucose detection. J Mater Chem A 2:7306–7312
Tyagi M, Tomar M, Gupta V (2014) Glad assisted synthesis of NiO nanorods for realization of enzymatic reagentless urea biosensor. Biosens Bioelectron 52:196–201
Xia KD, Yang C, Chen YL, Tian LL, Su YY, Wang JB, Li L (2017) In situ fabrication of Ni(OH)2 flakes on Ni foam through electrochemical corrosion as high sensitive and stable binder-free electrode for glucose sensing. Sensors Actuators B 240:979–987
Niu XH, Li X, Pan JM, He YF, Qiu FX, Yan YS (2016) Recent advances in non-enzymatic electrochemical glucose sensors based on non-precious transition metal materials: opportunities and challenges. RSC Adv 6:84893–84905
Liu MM, Liu R, Chen W (2013) Graphene wrapped Cu2O nanocubes: non-enzymatic electrochemical sensors for the detection of glucose and hydrogen peroxide with enhanced stability. Biosens Bioelectron 45:206–212
Wang L, Lu XP, Wen CJ, Xie YZ, Miao LF, Chen SH, Li HB, Li P, Song YH (2015) One-step synthesis of Pt-NiO nanoplate array/reduced graphene oxide nanocomposites for nonenzymatic glucose sensing. J Mater Chem A 3:608–616
Li M, Bo XJ, Mu ZC, Zhang YF, Guo LP (2014) Electrodeposition of nickel oxide and platinum nanoparticles on electrochemically reduced graphene oxide film as a nonenzymatic glucose sensor. Sensors Actuators B Chem 192:261–268
Soomro RA, Ibupoto ZH, Sirajuddin, Willander M (2015) Electrochemical sensing of glucose based on novel hedgehog-like NiO nanostructures. Sens Actuators B 209:966–974
Ding Y, Liu YX, Zhang LC, Wang Y, Bellagamba M, Parisi J, Li CM, Lei Y (2011) Sensitive and selective nonenzymatic glucose detection using functional NiO-Pt hybrid nanofibers. Electrochim Acta 58:209–214
Ding Y, Wang Y, Su LA, Zhang H, Lei Y (2010) Preparation and characterization of NiO-Ag nanofibers, NiO nanofibers, and porous Ag: towards the development of a highly sensitive and selective non-enzymatic glucose sensor. J Mater Chem 20:9918–9926
Reddy YAK, Ajitha B, Reddy PS, Reddy MSP, Lee JH (2014) Effect of substrate temperature on structural, optical and electrical properties of sputtered NiO-Ag nanocrystalline thin films. Electron Mater Lett 5:907–913
Li CC, Liu YL, Li LM, Du ZF, Xu SJ, Zhang M, Yin XM, Wang TH (2008) A novel amperometric biosensor based on NiO hollow nanospheres for biosensing glucose. Talanta 77:455–459
Ding Y, Wang Y, Zhang LC, Zhang H, Lei Y (2012) Preparation, characterization and application of novel conductive NiO-CdO nanofibers with dislocation feature. J Mater Chem 22:980–986
Zhang XJ, Gu AX, Wang GF, Huang Y, Ji HQ, Fang B (2011) Porous Cu-NiO modified glass carbon electrode enhanced nonenzymatic glucose electrochemical sensors. Analyst 136:5175–5180
This work was financially supported by the National Natural Science Foundation of China (21403020, 51503022), Basic and Frontier Research Program of Chongqing Municipality (cstc2016jcyjAX0014, cstc2016jcyjA0367, cstc2015jcyjA50036, CSTC2015JCYJBX0126, CSTC2016SHMSZX20001), Scientific and Technological Research Program of Chongqing Municipal Education Commission (KJ1601133, KJ1601104), Open Foundation of State Key Laboratory of Electronic Thin Films and Integrated Devices (KFJJ201507), and Chongqing University of Arts and Sciences (M2017ME20).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
He, G., Tian, L., Cai, Y. et al. Sensitive Nonenzymatic Electrochemical Glucose Detection Based on Hollow Porous NiO. Nanoscale Res Lett 13, 3 (2018). https://doi.org/10.1186/s11671-017-2406-0
- Hollow porous architecture
- Coordinating etching and precipitating
- Electrochemical sensor
- Glucose detection